Carbohydrate Polymers 101 (2014) 1122–1133
Contents lists available at ScienceDirect
Carbohydrate Polymers journal homepage: www.elsevier.com/locate/carbpol
Nano-biocomposite ﬁlms with modiﬁed cellulose nanocrystals and synthesized silver nanoparticles E. Fortunati a,∗ , S. Rinaldi b,1 , M. Peltzer c , N. Bloise d,e , L. Visai d,e , I. Armentano a , A. Jiménez c , L. Latterini b , J.M. Kenny a,f a
Materials Engineering Center, UdR INSTM, University of Perugia, Strada Pentima Bassa 4, 05100 Terni, Italy Dipartimento di Chimica and Centro di Eccellenza sui Materiali Innovativi Nanostrutturati (CEMIN), University of Perugia, Via Elce di Sotto 8, 06123 Perugia, Italy c University of Alicante, Department of Analytical Chemistry, Nutrition and Food Sciences, P.O. Box 99, 03080 Alicante, Spain d Department of Molecular Medicine, UdR INSTM, University of Pavia, 27100 Pavia, Italy e Department of Occupational Medicine, Ergonomics and Disability, Salvatore Maugeri Foundation, IRCCS, Laboratory of Nanotechnonolgy, Via S. Maugeri 8, 27100 Pavia, Italy f Institute of Polymer Science and Technology, CSIC, Calle Juan De La Cierva, 3, 28028 Madrid, Spain b
a r t i c l e
i n f o
Article history: Received 2 September 2013 Received in revised form 30 September 2013 Accepted 10 October 2013 Available online 23 October 2013 Keywords: Nano-biocomposites Cellulose nanocrystals Silver nanoparticles Barrier properties Migration properties Antibacterial activity
a b s t r a c t Ternary nano-biocomposite ﬁlms based on poly(lactic acid) (PLA) with modiﬁed cellulose nanocrystals (s-CNC) and synthesized silver nanoparticles (Ag) have been prepared and characterized. The functionalization of the CNC surface with an acid phosphate ester of ethoxylated nonylphenol favoured its dispersion in the PLA matrix. The positive effects of the addition of cellulose and silver on the PLA barrier properties were conﬁrmed by reductions in the water permeability (WVP) and oxygen transmission rate (OTR) of the ﬁlms tested. The migration level of all nano-biocomposites in contact with food simulants were below the permitted limits in both non-polar and polar simulants. PLA nano-biocomposites showed a signiﬁcant antibacterial activity inﬂuenced by the Ag content, while composting tests showed that the materials were visibly disintegrated after 15 days with the ternary systems showing the highest rate of disintegration under composting conditions. © 2013 Elsevier Ltd. All rights reserved.
1. Introduction Polymer nanocomposites have attracted considerable attention in recent years as a result of their good performance, improved properties, design ﬂexibility, lower life-cycle costs and a unique large applicability range in various industrial ﬁelds. Antimicrobial materials and surfaces are increasing their importance in areas such as healthcare, food active packaging, automotive and textiles to control harmful microorganisms (Hojatollah Bodaghi et al., 2013; Kuorwel et al., 2013; Manso, Cacho-Nerin, Becerril, & Nerín, 2013). However, all these systems need to combine a strong antibacterial efﬁciency with other characteristics, such as environmental safety, low toxicity, cost effectiveness and easy fabrication. Silver is a powerful antimicrobial agent that has been used since ancient times. Recent technical innovations facilitate the
∗ Corresponding author. Tel.: +39 0744 492921; fax: +39 0744 492950. E-mail address: [email protected]
(E. Fortunati). 1 Present address: Dipartimento di Chimica, Università di Siena, Via A. De Gasperi 2 (Quartiere di S. Miniato), 53100 Siena, Italy. 0144-8617/$ – see front matter © 2013 Elsevier Ltd. All rights reserved. http://dx.doi.org/10.1016/j.carbpol.2013.10.055
incorporation of silver-based materials to commercial formulations with antimicrobial properties (Fortunati, Latterini, Rinaldi, Kenny, & Armentano, 2011; Nocchetti et al., 2013; Rinaldi et al., 2013). Nanotechnology is one of the preferred innovations, allowing metals to be processed in the nanoscale to improve their chemical, physical and electronic properties (Busolo, Fernández, Ocio, & Lagaron, 2010; Lloret, Picouet, & Fernández, 2012). The synthesis of metallic nanoparticles with controlled shape, size and dispersion stability is a challenging research area due to their potential in electronics, optical, sensors and catalysis sectors (Cai, Kimura, Wada, & Kuga, 2009; Latterini & Tarpani, 2011; Storti, Elisei, Abbruzzetti, Viappiani, & Latterini, 2009). Preparation of metal colloids by reduction is a nominally simple reaction, but it requires a careful control of the synthesis conditions, since this process is sensitive to a balance between nucleation and crystal growth (Cai et al., 2009). This is a fundamental point since difﬁculties in dispersion of nanoparticles in a solvent are well known by their tendency to aggregate due to their high surface energy (Ifuku, Tsuji, Morimoto, Saimoto, & Yano, 2009). Silver ions are active against a very broad spectrum of bacteria, yeast, fungi and viruses even at very low concentration
E. Fortunati et al. / Carbohydrate Polymers 101 (2014) 1122–1133
˜ (Lara, Ayala-Nunez, Ixtepan-Turrent, & Rodriguez-Padilla, 2010; Nocchetti et al., 2013) with negligible toxicity towards human cells at the same concentration range (Williams, Doherty, Vince, Grashoff, & Williams, 1989). Moreover, colloidal nanosilver shows antimicrobial properties against Gram-positive and Gram-negative bacteria (Dallas, Sharma, & Zboril, 2011). These properties are particularly interesting for food active packaging (Lopez-Rubio, Lagaron, & Ocio, 2008). In the United States, the Center for Food and Drug Administration (FDA/CFSAN) accepts the use of silver nitrate as a food additive in bottled water. In addition to this, the European Food Safety Authority (EFSA) has concluded that there is no safety concern for the consumer if migration of silver ion does not exceed the group speciﬁc migration limit of 0.05 mg Ag kg−1 food (http://www.efsa.europa.eu/en/efsajournal/pub/1999.htm, updated 02 March 2011). Recent studies have reported that migration levels of silver nanoparticles in poly(vinyl chloride) (PVC) nanocomposites are clearly below the conventional migration limits indicated in the current European legislation (Reglament N10/2011) but the effects of nanoscale particles remain unclear and further studies are necessary to assess the real possibilities of nano-Ag in food packaging applications (Cushen, Kerry, Morris, Cruz-Romero, & Cummins, 2013). Nowadays, there is a trend to substitute petroleum based plastics by renewable plastic packaging with lower environment impact. In food packaging, PLA is a very promising material due to its excellent mechanical properties, transparency and commercial availability. Nonetheless, some of its properties, such as gas and water vapour permeability and thermal stability, are somewhat poor for some speciﬁc applications (Averous, Bordes, & Pollet, 2009). In this context, the addition of nanoparticles as polymer additives contributes to enhance the barrier to gases due to the synergistic tortuosity, crystal nucleation and chain immobilization effects (Martino, Ruseckaite, Jiménez, & Averous, 2010). Cellulose nanostructures have been recognized as important bio-based ﬁllers to enhance the biopolymer performance, in terms of mechanical, thermal and barrier properties (Fortunati, Peltzer, et al., 2012; Fortunati, Puglia, et al., 2013). Cellulose-based materials are widely used because of their biocompatibility, edibility, abundance in nature, excellent barrier properties and low cost (Brinchi, Cotana, Fortunati, & Kenny, 2013). The use of nanocelluloses has been widely proposed to enhance PLA properties (Bitinis et al., 2013; Frone, Berlioz, Chailan, & Panaitescu, 2012; Raquez et al., 2012). The aim of this research was the design, develop and characterize an innovative nano-biocomposite based on PLA, surfactant-modiﬁed cellulose nanocrystals (s-CNC) and synthesized silver nanoparticles (Ag) to be applied for fresh food antimicrobial active packaging. The effect of cellulose crystal nano-dimensions and the combination of cellulose nanostructures with synthesized silver nanoparticles were evaluated in terms of microstructure, crystallinity, water and oxygen barrier, migration and antibacterial properties. Moreover, the post-use properties of the developed multifunctional formulations were evaluated by a laboratory-scale composting condition test.
10–15 m) was supplied by Sigma–Aldrich (Milan, Italy). AgNO3 (Sigma–Aldrich, ACS reagent, ≥99.0%), polyvinylpyrrolidone (PVP, Mw = 40 kDa, Sigma–Aldrich), chloroform (CHCl3 , 99.4% GC-grade) were used as received. 2.2. Cellulose nanocrystals synthesis and modiﬁcation MCC was hydrolyzed in sulphuric acid (64%, wt/wt) at 45 ◦ C for 30 min (Fortunati, Peltzer, et al., 2012). Modiﬁed cellulose nanocrystals (s-CNC) were obtained after the addition of an acid phosphate ester of ethoxylated nonylphenol (Beycostat A B09 (CECCA S.A.)) in 1/4 (wt/wt) ratio as previously reported (Fortunati, Armentano, Zhou, Iannoni, et al., 2012; Fortunati, Armentano, Zhou, Puglia, et al., 2012). 2.3. Silver nanoparticles synthesis and characterization Silver nanoparticles (Ag) were synthesized by selective reduction in the presence of PVP to control the particle growth. AgNO3 (0.0856 g) was added to 50 mL of a CHCl3 boiling solution containing 0.72 g of PVP. The solution was then heated up to the boiling point and maintained at this temperature for 5 h under vigorous stirring. A Philips mod. 208 transmission electron microscope (TEM), operating at 80 kV of beam acceleration was used to analyze the average size and distribution of the silver nanoparticles. They were deposited in a 400 mesh copper coated with formvar support grid and were left overnight in a desiccator to evaporate the solvent. Histograms for size distribution were obtained by analyzing 150–200 nanoparticles in each sample. UV–vis absorption spectra of the Ag suspensions were recorded with a double beam Perkin-Elmer Lambda 800 spectrophotometer. 2.4. PLA nano-biocomposites processing
PLA nano-biocomposite ﬁlms were prepared by solvent casting. PLA was dissolved in CHCl3 (10%, wt/v) with vigorous stirring at room temperature (RT). The solutions were poured onto glass Petri dishes, and then allowed to dry for about 24 h at RT. PLA neat ﬁlms (200 ± 50) m thick were obtained (ﬁlm thickness was measured using a micrometre to ±0.001 mm, and ﬁve different measurements were performed). For the preparation of the nanocomposite ﬁlms, a predetermined amount of s-CNC suspension in chloroform was mixed with the previously prepared PLA solution. The obtained solutions were stirred for 4 h before they were cast onto glass Petri dishes and dried. The produced ﬁlms were (200 ± 50) m thick (ﬁlm thickness was measured using a micrometre to ±0.001 mm). Ternary ﬁlms with 0.5 wt% or 1 wt% of Ag combined with 1 wt% of s-CNC (designed as PLA/1s-CNC/0.5Ag and PLA/1s-CNC/1Ag, respectively) were produced and characterized. For comparison, binary PLA/Ag systems with 0.5 wt% or 1 wt% of Ag were also prepared and designed as PLA/0.5Ag and PLA/1Ag, respectively. Films with thicknesses of (200 ± 50) m were obtained (ﬁlm thickness was measured using a micrometre to ±0.001 mm). All ﬁlms were placed in a vacuum oven at 40 ◦ C for 2 weeks before characterization in order to remove remaining chloroform.
2.5. PLA nano-biocomposites characterization
Poly(lactic acid), PLA, 3051D, with speciﬁc gravity 1.25 g cm−3 , molar mass 1.42 × 104 g mol−1 and melt ﬂow index (MFI) 7.75 g 10 min−1 (210 ◦ C, 2.16 kg) was supplied by Nature Works® (Minnetonka, MN, USA). PLA resin 3051D had 96% l-lactide to 4% d-lactide units. PLA pellets were dried in a vacuum oven at 98 ◦ C for 3 h before processing. Microcrystalline cellulose (MCC, dimensions
2.5.1. Microstructure, transparency and Wide Angle X-ray Scattering (WAXS) The microstructure of PLA nano-biocomposites and the ﬁller dispersion in the matrix were investigated by using transmission electron microscope (TEM, JEOL JEM-2010). Samples for TEM analysis were previously ultra-microtomed (RMC, model MTXL) in order
E. Fortunati et al. / Carbohydrate Polymers 101 (2014) 1122–1133
to obtain slices 100 nm thick. A confocal laser scanning microscope (CLSM, Nikon PCM2000, Italy), equipped with a diode laser ( = 400 nm) or an Ar-laser ( = 488 nm) as light sources, was used to investigate the nanocomposite morphology and the nanoparticle dispersion. The absorption spectra of the ﬁlm samples were recorded with a Varian (Cary 4000, USA) spectrophotometer equipped with a 150 mm integration sphere for reﬂectance spectra recording. A bar of barium sulphate was used as reference to calibrate the spectrophotometer. Wide Angle X-ray Scattering (WAXS) patterns of PLA nanobiocomposites were obtained with a Seifert diffractometer (JSO-DEBYEFLEX 2002) with CuK radiation ( = 0.1546 nm), 40 kV voltage and 40 mA current. The diffraction intensities were recorded between 2◦ and 80◦ (2 angle range) by steps of 1◦ min−1 . 2.5.2. Thermal characterization Differential scanning calorimetry (DSC, Mettler Toledo 822e) measurements were performed from −25 ◦ C to 210 ◦ C, at 10 ◦ C min−1 (the samples were rapidly cooled to the start temperature), performing two heating and one cooling scans (210 ◦ C to −25 ◦ C at 10 ◦ C/min). Melting and cold crystallization temperatures and enthalpies (Tm (◦ C), Tcc (◦ C), Hm (J g−1 ), Hcc (J g−1 )) were determined from the second heating scan as well as glass transition temperatures (Tg (◦ C)) for all nano-biocomposites. 2.5.3. Oxygen transmission rate (OTR) measurements OTR values were determined by using an oxygen permeation analyzer (Systech Instruments, model 8500, Metrotec S.A., Spain). Film thicknesses were measured with a Digimatic Micrometer Series 293 MDC-Lite (Mitutoyo) to ±0.001 mm. Samples were clamped in the diffusion chamber at (25 ± 1) ◦ C. Pure oxygen (99.9%) was introduced into the upper half of the sample chamber while nitrogen was injected into the lower half of the chamber where an oxygen sensor was placed. Oxygen transmission rate per thickness (OTR*e) was determined for each formulation. 2.5.4. Water vapour permeability (WVP) tests Water vapour permeability was calculated by following the UNE-ISO 53097:2002 standard and according to the following equation: WVP (kg m/m2 s Pa) =
WVT ×e S × (RH1 − RH2 )
where e is the ﬁlm thickness (m), S is the saturation pressure (Pa) at the testing temperature, RH1 is the relative humidity of the climatic chamber where tests were performed and RH2 is the relative humidity inside the capsule. At least three repetitions per experiment were performed as previously reported (Martucci & Ruseckaite, 2010). Samples with a diameter of 95 mm were ﬁxed with parafﬁn to the top of aluminium capsules containing CaCl2 as drying agent. These capsules were placed in a climatic chamber at 20.0 ± 0.1 ◦ C and 50 ± 2% relative humidity. Samples were weighed periodically until the steady state was reached. The mass change (±0.0001 g) versus time was recorded at speciﬁc intervals (t) and then plotted. Linear regression was used to calculate the slope of the ﬁtted straight line, which represents WVT as follows: m WVT = t×A
where m is the mass change of the capsule test (kg) at time t (s) and A is the test area (m2 ). WVT (kg s−1 m−2 ) is the vapour transmission rate through a mean ﬁlm thickness e (m).
2.6. Overall and speciﬁc migration tests: kinetics of silver release In order to determine the overall migration of the samples under study, rectangular strips of 10 cm2 total area of each ﬁlm were immersed in glass tubes with 10 mL of ethanol 10% (v/v) (simulant A) and isooctane (alternative simulant to D2). Food simulants are used to demonstrate the compliance of plastic materials not yet in contact with food (Commission Regulation EU 10/2011). Samples in ethanol 10% (v/v) were kept in a controlled chamber at 40 ◦ C during 10 days according to the Regulation EU No. 10/2011 (Commission Regulation EU 10/2011), while samples in isooctane were kept at 20 ◦ C during 2 days, according to the EN 1186-1:2002 (European Standard EN 1186-1:2002). After the incubation period, ﬁlms were removed and simulants were evaporated to complete dryness. Furthermore, residues were weighed with an analytical balance (Sartorius ATILON) to ±0.1 mg in order to determine the overall migration value in mg kg−1 of simulant. Three independent determinations were performed for each sample and the ﬁnal overall migration value was the average of the three determinations. The same food simulants, ethanol 10% (v/v) and isooctane, were used to carry out the speciﬁc migration tests. In this case, rectangular strips of 12 cm2 total area of each ﬁlm were immersed in glass tubes with 20 mL of simulants to keep the relation 6 dm2 L−1 as indicated by the EN 13130 standard. Samples in ethanol 10% (v/v) were kept in a controlled atmosphere at 40 ◦ C for 10 days, while samples in isooctane were kept at 20 ◦ C for 2 days. After the incubation period, ﬁlms were removed and simulants were treated to determine the Ag+ amount. Prior to analysis isooctane extracts were evaporated to dryness and re-suspended in 5 mL of HNO3 1% (wt/v). Ethanol extracts were analyzed with no previous treatment. The determination of Ag in the migration extracts was performed by using Inductive Coupled Plasma spectroscopy with Mass Spectrometry detection (ICP-MS) model 7700× Agilent (Santa Clara, CA, USA) in argon (0.35 L min−1 ) at 1600 W radiofrequency and S/C temperature 2 ◦ C. The calibration curve was obtained with Ag+ standards in HNO3 1% (wt/v), in a concentration range between 5 g kg−1 and 1000 g kg−1 . Each standard was analyzed by triplicate. A release kinetics study was also performed in ethanol 10% (v/v) for 20 days to study the gradual release of Ag+ to the simulant at 40 ◦ C (Fortunati, Peltzer, Armentano, Jiménez, & Kenny, 2013). Diffusion coefﬁcients were calculated from the beginning of the release process by using a mathematical model based on the Fick’s second law. In this study, we propose the use of a simpliﬁed release model described by Eqs. (3) and (4), which are based on the Crank equation (Crank & Gupta, 1975) and described by Chung, Papadakis, and Yam (2002) where MP,0 is the initial amount of analyte in the polymer matrix and MF,t is the amount of migrant transferred from the ﬁlm to the food simulant from time zero to time t (s).
MF,t 2 Dt = MP,0 LP
KFP VF VP
D is the diffusion coefﬁcient (cm s−1 ) and Lp is the ﬁlm thickness. 2.7. Antibacterial activity The microorganisms used in this study were Escherichia coli RB (E. coli RB) and Staphylococcus aureus 8325-4 (S. aureus 83254). E. coli RB was provided by the “Zooproﬁlattico Institute of Pavia”, Italy whereas S. aureus 8325-4 was kindly supplied by Timothy J. Foster (Department of Microbiology, Dublin, Ireland).
E. Fortunati et al. / Carbohydrate Polymers 101 (2014) 1122–1133
E. coli RB was routinely grown in Luria Bertani Broth (LB) (Difco, Detroit, MI, USA) and S. aureus 8325-4 in Brian Heart Infusion (BHI) (Difco) overnight under aerobic conditions at 37 ◦ C using a shaker incubator (New Brunswick Scientiﬁc Co., Edison, NJ, USA). These cultures, used as source for the experiments, were reduced at a ﬁnal density of 1 × 1010 cells mL−1 as determined by comparing the OD600 of the sample with a standard curve relating OD600 to cell number. To evaluate the antimicrobial activity of PLA and PLA nanobiocomposite ﬁlms, 100 L (1 × 104 ) of overnight diluted cell suspensions of E. coli RB or S. aureus 8325-4 were added to each sample seeded at the bottom of 96-well tissue culture plates and incubated at different temperatures (37 ◦ C, 24 ◦ C and 4 ◦ C) for 3 h and 24 h, respectively. These temperatures were chosen to evaluate their inﬂuence on the antibacterial activity exerted by PLA and PLA nano-biocomposite ﬁlms as food packaging systems. Some food is kept refrigerated at 4 ◦ C but it may be possible that under transportation food could be kept at higher storage temperatures (24 ◦ C and/or 37 ◦ C). Furthermore, 96-well ﬂat-bottom sterile polystyrene culture plates (TCP), used as control, were incubated at the same temperatures and times. At the end of each incubation period, the bacterial suspension was then serially diluted, and plated on the LB (E. coli) or BHI (S. aureus) agar plates, respectively. Those plates were then incubated for 24 h/48 h at 37 ◦ C. Cell survival was expressed as percentage of the CFU of bacteria survived on PLA nano-biocomposite ﬁlms to CFU of bacteria grown on PLA and PLA/1s-CNC without Ag. Further analysis of the antibacterial activity of these samples was carried out by determining the release of Ag+ with a PerkinElmer series ICP-MS, analysing those solutions obtained by the interaction of solvent with samples (area 1 cm2 ) at 37 ◦ C at 3 different incubation times (3 h, 24 h and 72 h). Solutions were regularly analyzed by ICP-MS to determine the concentration of Ag+ , once the instrumental setup had been calibrated with a standard solution. Experiments were conducted in duplicate. 2.8. Disintegrability in composting conditions Disintegrability of PLA and PLA nano-biocomposites was followed through a disintegration test in composting conditions according to the ISO-20200 standard. A speciﬁc quantity of compost, supplied by Gesenu S.p.a. (Italy), was mixed together with the synthetic biowaste, prepared with certain amount of sawdust, rabbit food, starch, sugar, oil and urea. The water content of the substrate was around 50 wt% and the aerobic conditions were guaranteed by mixing it softly. The samples were buried at 4–6 cm depth in perforated boxes, containing the prepared mix, and incubated at 58 ◦ C. The (20 mm × 20 mm × 0.02 mm) ﬁlms were recovered at different disintegration steps, washed with distilled water, dried in oven at 37 ◦ C for 24 h, and weighed. The disintegrability value was obtained normalizing the sample weight, at different stages of incubation, to the initial ones. Photographs of the samples were taken for visual comparison.
3. Results and discussion 3.1. Surfactant modiﬁed cellulose nanocrystals Fig. 1 (panel A) summarizes the different steps and strategies used to prepare cellulose based nano-biocomposites in this study. Cellulose nanocrystals are recovered in water suspension after acid hydrolysis and the TEM micrograph (left side of the scheme) shows that CNC appears well individualized with typical dimensions ranging from 100 to 200 nm in length and 5–10 nm in width as previously reported (Fortunati, Armentano, Zhou, Iannoni, et al., 2012; Fortunati, Armentano, Zhou, Puglia, et al., 2012). Because of the high stability of aqueous cellulose nanoparticle suspensions, water is the preferred medium to prepare nanocomposite ﬁlms. However, this fact restricts the choice of the matrix to hydrosoluble polymers, which are inherently highly sensitive to humidity. In recent works we demonstrated that the freeze-drying step is critical for the production of nano-biocomposites with uniform cellulose nanocrystal dispersion since the CNC tend to agglomerate into ﬂakes during the freeze-drying (see Fig. 1, panel A) (Fortunati, Armentano, Zhou, Iannoni, et al., 2012; Fortunati, Armentano, Zhou, Puglia, et al., 2012). The use of surfactants to obtain a stable suspension of cellulose nanocrystals in organic media is a procedure used by different authors (Ljungberg et al., 2005; Petersson, Kvien, & Oksman, 2007). The surfactant used in this research is able to hinder hydrogen bonding between the cellulose nanocrystals during the freeze drying and to further increase the distribution of cellulose in organic solvents, such as chloroform (Averous et al., 2009). The FESEM image shown in Fig. 1 (panel A), right highlights the crystal shape and size of surfactant modiﬁed cellulose (s-CNC): cellulose nanocrystals maintained the original acicular structure and no morphological modiﬁcations occurred during the dispersion in the organic solvent. 3.2. Silver nanoparticle characterization The chemical synthesis of silver nanoparticles (Ag) was carried out in chloroform, in order to obtain a particle suspension within the same solvent used for PLA. The preparation of Ag particles in CHCl3 was carried out following a previously reported procedure (Rinaldi et al., 2013). The formation of Ag was monitored spectrophotometrically in the reaction solutions. The presence of an intense absorption band centred at 430 nm in the extinction spectrum (Fig. 1, panel B-a), which was assigned to the surface plasmon resonance band of Ag, conﬁrmed the formation of silver colloids in CHCl3 . TEM was used to obtain information on the size and morphology of metal nanostructures. Fig. 1, panel B-b shows that the obtained suspensions were characterized by spherical silver nanoparticles, with no aggregates. The statistical analysis of nanoparticle diameter indicated a Gaussian distribution, centred at (7.8 ± 0.4) nm with (1.1 ± 0.1) nm as full width at half maximum (FWHM), indicating a good dispersion.
2.9. Statistical analysis
3.3. PLA nano-biocomposites: microstructure, transparency and WAXS analyses
S. aureus and E. coli cells grown on PLA were used as positive controls. Continuous data were expressed as the average and standard deviations (SD). Two-group comparisons were performed by application of the Student’s t test. All analyses were performed by using GraphPad Prism 4.0 (Graph Pad Software Inc., San Diego, CA, USA). Two-tailed p values p). (b). Ag release upon degradation of PLA nano-biocomposite ﬁlms. The Ag+ ions release was detected on the same samples incubated in physiological conditions at 37 ◦ C for 3 h, 24 h and 72 h, respectively. Results are expressed on a biomaterial-basis and are presented as an average ± standard deviation.
E. Fortunati et al. / Carbohydrate Polymers 101 (2014) 1122–1133
Fig. 7. (a) PLA and PLA nano-biocomposites before (0 days) and after different stages of disintegration in composting at 58 ◦ C. (b) Disintegrability percentage values of PLA and PLA nano-biocomposites at different stages of incubation in composting.
3.7. Antibacterial properties Fig. 6a shows the viability of E. coli (Fig. 6a-A and a-B) and S. aureus (Fig. 6a-C and a-D) cells onto PLA nano-biocomposite ﬁlms after 3 h and 24 h incubation at 4 ◦ C, 22 ◦ C and 37 ◦ C, respectively. As expected, the cell viability for both bacterial strains on PLA and PLA/1s-CNC ﬁlms without Ag nanoparticles was quite similar at each incubation time and temperature (data not shown) (p > 0.05). On the contrary, PLA and PLA/1s-CNC ﬁlms enriched with different concentrations of Ag nanoparticles (0.5 wt% or 1 wt%) showed an Ag dose-dependent antibacterial activity against E. coli and S. aureus strains but with some differences. The antibacterial activity was greater on E. coli than on S. aureus cells regardless of the incubation times and temperatures. These results are in agreement with previous studies showing that Ag nanoparticles are more toxic to E. coli than to S. aureus (Li et al., 2010; Wen-Ru et al., 2011). The reduced antibacterial activity on PLA nano-biocomposites for S. aureus may be due to the structural difference in the cell wall of Gram-positive if compared to Gram-negative cells. In fact, since the thick peptidoglycan layer of the staphylococcal cell wall prevents the penetration of the nanoparticles inside the cytoplasm, the antimicrobial effect is limited and seems related to the interaction with the bacterial surfaces or to the capture of the released silver ions. Only once inside the bacterial cell, the Ag+ ions are known to interact with thiol groups of the proteins and to inactive the enzyme activity (Liau, Read, Pugh, Furr, & Russel, 1997); silver ions turning DNA into a condensed form leading to the damage or even the death of the microorganisms (Kim et al., 2007). Recent studies showed that Ag nanoparticles in the range of 5–20 nm could more easily reach the nuclear content of bacteria by disrupting their membranes and increasing bacterial killing (Bin Ahmad et al., 2012; Lu, Rong, Li, Yang, & Chen, 2013). As regards the incubation time, the percentage of bacterial surviving fraction was higher after 3 h (Fig. 6a-A and a-C) if compared to a longer incubation time (24 h, Fig. 6a-B and 6a-D) for both bacterial strains (0.05 > p). The percentage of cell viability for both bacterial strains was slightly dependent on the incubation temperature and time: the cell surviving fraction was more reduced at 37 ◦ C if compared at 22 ◦ C and 4 ◦ C after 24 h incubation time (Fig. 6B and D) (0.05 < p). This effect was less evident after 3 h (Fig. 6a-A and a-C). The antibacterial activity was also dependent on the Ag content, showing the highest value for samples containing 1 wt% Ag. These results are conﬁrmed by previous studies performed on different PLA nano-biocomposites with higher Ag contents (Shameli et al., 2010). In addition, the antibacterial activity was signiﬁcantly higher in the presence of 1 wt% s-CNC (0.05 > p) for both strains incubated at 37 ◦ C for 24 h. Fig. 6b shows the release of Ag+ ions from PLA nano-biocomposite ﬁlms in
physiological conditions at 37 ◦ C: even if the ions release was quite low, it was more evident for PLA nano-biocomposites containing 1s-CNC and reached their maximum after 24 h. These results were in agreement with the migration kinetics previously discussed. The higher release of Ag+ ions from PLA/1s-CNC samples may explain their greater antibacterial activity on both strains at 37 ◦ C after 24 h if compared to PLA/Ag samples at the same incubation time and temperature. In summary, the antibacterial activity for both strains was stronger on PLA/1s-CNC containing 1 wt% Ag nanoparticles if compared to PLA/1Ag when performed at longer incubation times. However, the effect was more signiﬁcant for E. coli cells if compared to S. aureus cells. 3.8. Disintegrability in composting conditions The biodegradation of PLA in compost is one of its most attractive properties for this polymer in massive applications, such as food packaging to limit the serious problem of waste disposal (Kale, Auras, Singh, & Narayan, 2007). The effect of nanoparticles on PLA biodegradation in compost has been reported over the past few years (Fukushima, Tabuani, Abbate, Arena, & Ferreri, 2010; Fortunati, Puglia, Santulli, Sarasini, & Kenny, 2012) and some delay in biodegradability of the biopolymer was observed. This effect is due to the improvement in water barrier properties of the nanobiocomposites, which could hinder the water diffusion through the bulk and consequently decrease the hydrolysis rate (Lee et al., 2002). The study of the disintegration in composting conditions of PLA nano-biocomposites was carried out to evaluate the effect of the addition of silver nanoparticles and s-CNC nanocrystals on the disintegrability properties of the PLA matrix. Fig. 7a shows photographs of all samples at different composting times. Whitening and deformation of the ﬁlms surface were detected just after the ﬁrst day of incubation for all materials and these effects were enhanced after 3 days in composting conditions. These results are indicative of the beginning of the hydrolytic degradation, which was faster than expected by the low thickness of ﬁlms (30–40 m). The loss of transparency observed for all samples could be attributed to changes in the refractive index due to the water absorption and the formation of low molecular weight compounds after the hydrolytic degradation (Fukushima et al., 2010). It has been indicated that the PLA hydrolysis begins in the amorphous region of the polymer structure and all these effects would also result in changes in the polymer crystallinity and consequently in loss of transparency (Zaidi, Kaci, Bruzaud, Bourmaud, & Grohens, 2010). Moreover, it should be taken into account that the degradation experiments took place at 58 ◦ C, which is higher than the Tg
0.005 0.005 0.18 0.22
1.50 × 10 8.50 × 10−17 2.50 × 10−14 2.3 × 10−14 0.7 0.24 0.8 1.0 1.0 1.1 7 11 ± ± ± ± 4.0 4.2 40 94
Ethanol 10% v/v (10 days, 40 ◦ C) (g kg−1 simulant)
149.8 ± 0.5 150.4 ± 0.2
of the matrix. This could increase the chain mobility, inducing the crystallization of the PLA matrix. At the 7th day, fragmentation and weight loss of the nano-biocomposites were already observed for all samples except for PLA neat ﬁlm, which started fragmentation after the 10th day. Fig. 7b shows the evolution of disintegrability values at different incubation times. It was observed that after 28 days of composting test, all materials reached 90% of disintegration. The addition of silver nanoparticles increased the degradation rate of PLA matrix reaching 60% at 10 days for PLA/0.5Ag and PLA/1Ag in comparison with 20% for the neat PLA ﬁlm. These results are in agreement with those reported by other authors in PLA nanocomposites (Fukushima et al., 2010; Paul et al., 2005). The addition of cellulose nanocrystals also increased the disintegrability rate, but lower values were detected at 7 and 10 days for the PLA/1s-CNC/0.5Ag and PLA/1s-CNC/1Ag ternary systems than those obtained for binary nano-biocomposites. This behaviour could be attributed to the double effect caused by the addition of a hydrophilic ﬁller, such as cellulose nanocrystals, which are expected to accelerate the degradation rate of the PLA nano-biocomposites. But, on the other hand, s-CNC could also limit the water diffusion by the increase in barrier properties and consequently delaying hydrolysis and further degradation. These results underlined that all the studied nanobiocomposites started the disintegration process before and with higher rate than neat PLA ﬁlms, suggesting their perspective advantages in industrial applications when short biodegradation times are required.
± ± ± ± 1.0 0.95 1.1 2.4
D (cm2 s−1 ) Isooctane (2 days, 20 ◦ C) (g kg−1 simulant)
39 44 43 63 0.18 0.07 0.09 0.08 0.01 ± ± ± ± ± 1.04 0.64 0.58 0.59 0.39 20 35 41 56 1.0 0.1 0.6 0.7 0.4 ± ± ± ± ± 30.5 24.3 19.7 18.1 13.4 115.9 ± 107.0 ± 100.5 ± 100.6 ± 0.3 0.1 0.2 0.9 16.4 ± 17.3 ± 17.3 ± 17.2 ± -
PLA/0.5Ag PLA/1Ag PLA/1s-CNC/0.5Ag PLA/1s-CNC/1Ag
PLA PLA/0.5Ag PLA/1Ag PLA/1s-CNC/0.5Ag PLA/1s-CNC/1Ag
45.0 52.6 49.5 49.3 48.6
± ± ± ± ±
2.0 1.1 0.1 1.2 0.4
25.8 24.1 25.4 27.7 27.8
± ± ± ± ±
0.7 0.4 0.4 0.7 0.1
151.2 147.2 145.4 143.1 143.4
± ± ± ± ±
0.5 0.2 0.1 0.1 0.3
(◦ C) Tm
Tm (◦ C) Hm (J/g) Tg (◦ C)
First heating scan
Thermal properties Samples
Table 1 Thermal, barrier and migration behaviour of PLA and PLA nano-biocomposites.
Tcc (◦ C)
1.2 0.8 2.0 0.3
OTR*e (cm3 mm m−2 day−1 )
Reduction in OTR (%)
WVP *1014 (kg ms−1 m2 Pa)
Reduction in WVP (%)
E. Fortunati et al. / Carbohydrate Polymers 101 (2014) 1122–1133
The high potential beneﬁts offered by nanotechnology in the development of tailor-made nano-biocomposites with speciﬁc applications is here shown by the combination of two different synthesized nanostructures: silver nanoparticles and cellulose nanocrystals in a biodegradable polymer matrix. Ternary nanobiocomposites based on PLA containing modiﬁed s-CNC and Ag nanoparticles were prepared by the solvent casting method and further characterized. Results showed the homogeneous particle dispersion in the polymer matrix, not affecting the original PLA transparency. The s-CNC induced PLA crystallization, which combined with the higher content of silver, resulted in clear enhancement of barrier properties to oxygen and water vapour (41% and 56% for PLA/1s-CNC/0.5Ag and PLA/1s-CNC/1Ag ternary nano-biocomposites, respectively). Reduction of about 40–45% in barrier properties was detected for binary systems, which was maximized for ternary systems loaded with 1 wt% of Ag, suggesting the positive effect of silver and its combination with cellulose nanostructures. Overall and speciﬁc migration values were well below the limits indicated by EFSA, while after the release of Ag+ to ethanol 10% (v/v) in ternary nano-biocomposites with 1 wt% of Ag exceeded the permitted limits. Higher migration was observed in those samples with cellulose, may be due to the interaction between the carbonyl groups PVP and the primary hydroxyl functionalities of cellulose that lead to the release of Ag+ . The addition of s-CNC resulted important for the improvement of the antibacterial activity of PLA/Ag. Finally the nanobiocomposites studied here started their disintegration process before and with a higher rate than pure PLA suggesting their perspective advantages in industrial applications when short biodegradation times are required. In summary, the combination of the antibacterial properties of silver nanoparticles with cellulose nanocrystals in the PLA shows high potential to improve functional active properties with important implications in the development of new biodegradable materials for fresh food packaging applications.
E. Fortunati et al. / Carbohydrate Polymers 101 (2014) 1122–1133
Acknowledgements L.V. would like to acknowledge the ﬁnancial support from MIUR, PRIN 2010–11 project entitled “Nanomed” (prot. 2010FPTBSH 009). M.P. and A.J. acknowledge the ﬁnancial support from the Spanish Ministry of Economy and Competitiveness (MAT2011-28648-C02-1). Authors acknowledge Gesenu S.p.a. for compost supply, which was necessary to obtain synthetic biowaste. References Alin, J., & Hakkarainen, M. (2011). Microwave heating causes rapid degradation of antioxidants in polypropylene packaging, leading to greatly increased speciﬁc migration to food simulants as shown by ESI-MS and GC–MS. Journal of Agricultural and Food Chemistry, 59, 5418–5427. Averous, L., Bordes, P., & Pollet, E. (2009). Nano-biocomposites: Biodegradable polyester/nanoclay systems. Progress in Polymer Science, 34, 125–155. Baia, L., Muresan, D., Baia, M., Popp, J., & Simon, S. (2007). Structural properties of silver nanoclusters–phosphate glass composites. Vibrational Spectroscopy, 43, 313–318. Bin Ahmad, M., Lim, J. J., Shameli, K., Ibrahim, N. A., Tay, M. Y., & Chieng, B. W. (2012). Antibacterial activity of silver bionanocomposites synthesized by chemical reduction route. Chemistry Central Journal, 6, 101–110. Bitinis, N., Verdejo, R., Bras, J., Fortunati, E., Kenny, J. M., Torre, L., et al. (2013). Poly(lactic acid)/natural rubber/cellulose nanocrystal bionanocomposites. Part I. Processing and morphology. Carbohydrate Polymers, 96, 611–620. Brinchi, L., Cotana, F., Fortunati, E., & Kenny, J. M. (2013). Production of nanocrystalline cellulose from lignocellulosic biomass: Technology and applications. Carbohydrate Polymers, 94, 154–169. Burgos, N., Martino, V. P., & Jiménez, A. (2013). Characterization and ageing study of poly(lactic acid) ﬁlms plasticized with oligomeric lactic acid. Polymer Degradation and Stability, 98, 651–658. Busolo, M. A., Fernández, P., Ocio, M. J., & Lagaron, J. M. (2010). Novel silver-based nanoclay as an antimicrobial in polylactic acid food packaging coatings. Food Additives and Contaminants: Part A, 27, 1617–1626. Cai, J., Kimura, S., Wada, M., & Kuga, S. (2009). Nanoporous cellulose as metal nanoparticles support. Biomacromolecules, 10, 87–94. Chung, D., Papadakis, S. E., & Yam, K. L. (2002). Simple models for assessing migration from food packaging ﬁlms. Food Additives and Contaminants, 19, 611–617. Commission Regulation (EU) No. 10/2011 of 14 January 2011 on plastic materials and articles intended to come into contact with food. Crank, J., & Gupta, R. S. (1975). Isotherm migration method in two dimensions. International Journal of Heat and Mass Transfer, 18, 1101–1107. Cushen, M., Kerry, J., Morris, M., Cruz-Romero, M., & Cummins, E. (2013). Migration and exposure assessment of silver from a PVC nanocomposite. Food Chemistry, 139, 389–397. Dallas, P., Sharma, V. K., & Zboril, R. (2011). Silver polymeric nanocomposites as advanced antimicrobial agents: Classiﬁcation, synthetic paths, applications, and perspectives. Advances in Colloid and Interface Science, 166, 119–135. EFSA. (2005). Opinion of the Scientiﬁc Panel on food additives, ﬂavourings, processing aids and materials in contact with food (AFC) on a request from the Commission related to a 7th list of substances for food contact materials. EFSA Journal, 201. Available from: http://www.efsa.europa.eu/en/scdocs/scdoc/201a.htm European Standard EN 1186-1:2002. Materials and articles in contact with foodstuffs: Plastics. Guide to the selection of conditions and test methods for overall migration. ˜ Fernández, A., Soriano, E., Hernández-Munoz, P., & Gavara, R. (2010). Migration of antimicrobial silver from composites of polylactide with silver zeolites. Journal of Food Science, 75, 186–193. Fortunati, E., Armentano, I., Iannoni, A., & Kenny, J. M. (2010). Development and thermal behaviour of ternary PLA matrix composites. Polymer Degradation and Stability, 95, 2200–2206. Fortunati, E., Armentano, I., Zhou, Q., Iannoni, A., Saino, E., Visai, L., et al. (2012). Multifunctional bionanocomposite ﬁlms of poly(lactic acid), cellulose nanocrystals and silver nanoparticles. Carbohydrate Polymers, 87, 1596–1605. Fortunati, E., Armentano, I., Zhou, Q., Puglia, D., Terenzi, A., Berglund, L. A., et al. (2012). Microstructure and nonisothermal cold crystallization of PLA composites based on silver nanoparticles and nanocrystalline cellulose. Polymer Degradation and Stability, 97, 2027–2036. Fortunati, E., Latterini, L., Rinaldi, S., Kenny, J. M., & Armentano, I. (2011). PLGA/Ag nanocomposites: In-vitro degradation study and silver ion release. Journal of Material Science: Materials in Medicine, 12, 2735–2744. Fortunati, E., Peltzer, M., Armentano, I., Jiménez, A., & Kenny, J. M. (2013). Combined effects of cellulose nanocrystals and silver nanoparticles on the barrier and migration properties of PLA nano-biocomposites. Journal of Food Engineering, 118, 117–124. Fortunati, E., Peltzer, M., Armentano, I., Torre, L., Jimenez, A., & Kenny, J. M. (2012). Effects of modiﬁed cellulose nanocrystals on the barrier and migration properties of PLA nano-biocomposites. Carbohydrate Polymers, 90, 948–956. Fortunati, E., Puglia, D., Luzi, F., Santulli, C., Kenny, J. M., & Torre, L. (2013). Binary PVA bio-nanocomposites containing cellulose nanocrystals extracted from different natural sources: Part I. Carbohydrate Polymers, 97, 825–836.
Fortunati, E., Puglia, D., Santulli, C., Sarasini, F., & Kenny, J. M. (2012). Biodegradation of Phormium tenax/poly(lactic acid) composites. Journal of Applied Polymer Science, 125, E562–E572. Frone, A. N., Berlioz, S., Chailan, J. F., & Panaitescu, D. M. (2012). Morphology and thermal properties of PLA–cellulose nanoﬁbers composites. Carbohydrate Polymers, 91, 377–384. Fukushima, K., Tabuani, D., Abbate, C., Arena, M., & Ferreri, L. (2010). Effect of sepiolite on the biodegradation of poly(lactic acid) and polycaprolactone. Polymer Degradation and Stability, 95, 2049–2056. Hojatollah Bodaghi, H., Mostoﬁ, Y., Oromiehie, A., Zamani, Z., Ghanbarzadeh, B., Costa, C., et al. (2013). Evaluation of the photocatalytic antimicrobial effects of a TiO2 nanocomposite food packaging ﬁlm by in vitro and in vivo tests. LWT – Food Science and Technology, 50, 702–706. Ifuku, S., Tsuji, M., Morimoto, M., Saimoto, H., & Yano, H. (2009). Synthesis of silver nanoparticles templated by TEMPO-mediated oxidized bacterial cellulose nanoﬁbers. Biomacromolecules, 10, 2714–2717. Kale, G., Auras, R., Singh, S. P., & Narayan, R. (2007). Biodegradability of polylactide bottles in real and simulated composting conditions. Polymer Testing, 26, 1049–1061. Kim, J. S., Kuk, E., Yu, K. N., Kim, J., Park, S. J., Lee, H. J., et al. (2007). Antimicrobial effects of silver nanoparticles. Nanomedicine: Nanotechnology, Biology and Medicine, 3, 95–101. Kuorwel, K., Kuorwel, K. K., Cran, M. J., Sonneveld, K., Miltz, J., & Bigger, S. W. (2013). Migration of antimicrobial agents from starch-based ﬁlms into a food simulant. LWT – Food Science and Technology, 50, 432–438. ˜ Lara, H. M., Ayala-Nunez, N. V., Ixtepan-Turrent, L., & Rodriguez-Padilla, C. (2010). Mode of antiviral action of silver nanoparticles against HIV-1. Journal of Nanobiotechnology, 8, 1–10. Latterini, L., & Tarpani, L. (2011). Hierarchical assembly of nanostructures to decouple ﬂuorescence and photothermal effect. Journal of Physical Chemistry C, 115, 21098–21104. Lee, S. R., Park, H. M., Lim, H., Kang, T. Y., Li, X. C., Cho, W. J., et al. (2002). Microstructure, tensile properties, and biodegradability of aliphatic polyester/clay nanocomposites. Polymer, 43, 2495–2500. Li, W. R., Xie, X. B., Shi, Q. S., Zeng, H. Y., Ou-Yang, Y. S., & Chen, Y. B. (2010). Antibacterial activity and mechanism of silver nanoparticles on Escherichia coli. Applied Microbiology and Biotechnology, 85, 1115–1122. Liau, S. Y., Read, D. C., Pugh, W. J., Furr, J. R., & Russell, A. D. (1997). Interaction of silver-nitrate with readily identiﬁable groups – Relationship to the antibacterial action of silver ions. Letters in Applied Microbiology, 25, 279–283. Ljungberg, N., Bonini, C., Bortolussi, F., Boisson, C., Heux, L., & Cavaille, J. Y. (2005). New nanocomposite material reinforced with cellulose whiskers in atactic polypropylene: Effect of surface and dispersion characteristics. Biomacromolecules, 6, 2732–2739. Lloret, E., Picouet, P., & Fernández, A. (2012). Matrix effects on the antimicrobial capacity of silver based nanocomposite absorbing materials. LWT – Food Science and Technology, 49, 333–338. Lopez-Rubio, A., Lagaron, J. M., & Ocio, M. J. (2008). Active polymer packaging of nonmeat food products. In J. Kerry, & P. Butler (Eds.), Smart packaging technologies for fast moving consumer goods (pp. 19–33). Chichester: Wiley. Lu, Z., Rong, K., Li, J., Yang, H., & Chen, R. (2013). Size-dependent antibacterial activities of silver nanoparticles against oral anaerobic pathogenic bacteria. Journal of Materials Science: Materials in Medicine, 24, 1465–1471. Manso, S., Cacho-Nerin, F., Becerril, R., & Nerín, C. (2013). Combined analytical and microbiological tools to study the effect on Aspergillus ﬂavus of cinnamon essential oil contained in food packaging. Food Control, 30, 370–378. Martino, V. P., Ruseckaite, R. A., Jiménez, A., & Averous, L. (2010). Correlation between composition, structure and properties of poly(lactic acid)/polyadipatebased nano-biocomposites. Macromolecular Materials & Engineering, 295, 551–558. Martucci, J. F., & Ruseckaite, R. A. (2010). Three-layer sheets based on gelatin and poly(lactic acid). Part 1. Preparation and properties. Journal of Applied Polymer Science, 118, 3102–3110. Masson, J. F., & Manley, R. (1991). Miscible blends of cellulose and poly(vinylpyrrolidone). Macromolecules, 24, 6670–6679. Nocchetti, M., Donnadio, A., Ambrogi, V., Andreani, P., Bastianini, M., Pietrella, D., et al. (2013). Ag/AgCl nanoparticle decorated layered double hydroxides: Synthesis, characterization and antimicrobial properties. Journal of Material Chemistry B, 1, 2383–2393. Paul, M. A., Delcourt, C., Alexandre, M., Degee, P., Monteverde, F., & Dubois, P. (2005). Polylactide/montmorillonite nanocomposites: Study of the hydrolytic degradation. Polymer Degradation and Stability, 87, 535–542. Pei, A., Zhou, Q., & Berglund, L. A. (2010). Functionalized cellulose nanocrystals as biobased nucleation agents in poly(l-lactide) (PLLA): Crystallization and mechanical property effects. Composites Science and Technology, 70, 815–821. Petersson, L., Kvien, I., & Oksman, K. (2007). Structure and thermal properties of poly(lactic acid)/cellulose whiskers nanocomposites materials. Composites Science and Technology, 67, 2535–2544. Petersson, L., & Oksman, K. (2006). Biopolymer based nanocomposites: Comparing layered silicates and microcrystalline cellulose as nanoreinforcement. Composites Science and Technology, 66, 2187–2196. Raquez, J. M., Murena, Y., Gofﬁn, A. L., Habibi, Y., Ruelle, R., DeBuyl, F., et al. (2012). Surface-modiﬁcation of cellulose nanowhiskers and their use as nanoreinforcements into polylactide: A sustainably-integrated approach. Composites Science and Technology, 72, 544–549.
E. Fortunati et al. / Carbohydrate Polymers 101 (2014) 1122–1133 Rinaldi, S., Fortunati, E., Taddei, M., Kenny, J. M., Armentano, I., & Latterini, L. (2013). Integrated PLGA–Ag nanocomposite systems to control the degradation rate and antibacterial properties. Journal of Applied Polymer Science, 130, 1185–1193. Schmidt, B., Katiyar, V., Plackett, D., Larsen, E. H., Gerds, N., Koch, B. C., et al. (2011). Migration of nanosized layered double hydroxide platelets from polylactide nanocomposite ﬁlms. Food Additives and Contaminants, 28, 956–966. Shameli, K., Ahmad, M. B., Yunus, W. M., Ibrahim, N. A., Rahman, R. A., Jokar, M., et al. (2010). Silver/poly (lactic acid) nanocomposites: Preparation, characterization, and antibacterial activity. International Journal of Nanomedicine, 5, 573–579. Storti, B., Elisei, F., Abbruzzetti, S., Viappiani, C., & Latterini, L. (2009). One-pot synthesis of gold nanoshells with high photon-to-heat conversion efﬁciency. Journal of Physical Chemistry C, 113, 7516–7521.
Wen-Ru, L., Xiao-Bao, X., Qing-Shan, S., Shun-Shan, D., You-Sheng, O., & Yi-Ben, C. (2011). Antibacterial effect of silver nanoparticles on Staphylococcus aureus. Biometals, 24, 135–141. Williams, R. L., Doherty, P. J., Vince, D. G., Grashoff, G. J., & Williams, D. F. (1989). The biocompatibility of silver. Critical Reviews in Biocomposites, 5, 221–243. Xiang, C., Taylor, A. G., Hinestroza, J. P., & Frey, M. W. (2013). Controlled release of non-ionic compounds from poly(lactic)/cellulose nanocrystals nanocomposite ﬁbers. Journal of Applied Polymer Science, 127, 79–86. Xiang, C. H., Joo, Y. L., & Frey, M. W. (2009). Nanocomposite ﬁbers electrospun from poly(lactic acid)/cellulose nanocrystals. Journal of Biobased Materials and Bioenergy, 3, 147–155. Zaidi, L., Kaci, M., Bruzaud, S., Bourmaud, A., & Grohens, Y. (2010). Effect of natural weather on the structure and properties of polylactide/Cloisite 30B nanocomposites. Polymer Degradation and Stability, 95, 1751–1758.